Brine compositions (wt%).
Supramolecular polymer networks are built up by combining multiple noncovalent interactions among macromolecules, resulting in the formation of materials with versatile functionality. This chapter describes an exploratory research focused on the formulation of a supramolecular polymer network based on reversible interactions among the main- and side chains of a mixture of xanthan gum, partly hydrolyzed polyacrylamide (HPAM), and a hydrophobically modified polyacrylamide (HMPAM) in brine solutions relevant for applications in enhanced oil recovery (EOR). The formation and characterization of the supramolecular network system was carried out through oscillatory rheology.
- supramolecular polymers
- polymer flooding
- heavy oil recovery
- salt tolerance
- mechanical stability
- thermal stability
Self-organization of molecular structures refers to the spontaneous assembly of individual building blocks into ordered and thermodynamically stable nanostructures by noncovalent interactions, resulting in the formation of dynamic and responsive materials. The noncovalent (reversible) interactions include electrostatic attractions, metal/ligand complexes, π/π-stacking, ionic interactions, hydrogen bonding, or hydrophobic effects without the application of external energy. Therefore, self-assembly is a low-cost and high-yield process [1, 2, 3, 4, 5, 6] that can be activated by external stimuli, which involves changes in temperature, pH, ionic strength, radiation, the addition of other molecules, or their combination [2, 7, 8, 9].
Supramolecular polymer networks can be formed by polymer blends (PBs) in which the reversible and highly directional noncovalent interactions are randomly distributed across the polymer chains . The resulting supramolecular structure displays polymeric properties in dilute and concentrated solutions that follow well-established theories of polymer physics . These networks exhibit enhanced material properties compared to the individual polymers , and the reversibility of noncovalent interactions provides self-healing properties to these materials [6, 10].
This study focuses on the formulation and characterization of a supramolecular polymer network based on reversible interactions among the main- and side chains of a mixture of xanthan gum, HPAM, and HMPAM or associating polymer (AP) in brine. Xanthan gum and HPAM are the most commonly used polymers in the field for enhanced oil recovery (EOR) . Figure 1 displays the chemical structures of these polymers.
Xanthan gum is a high-molecular weight (≈2–3 × 106 g/mol) anionic polysaccharide derived from the fermentation of the bacterium
Xanthan gum is a stereoregular polymer and displays order–disorder transition in solution that depends on polymer concentration, ionic strength, and temperature [11, 12, 13, 14, 17, 19, 24, 26]. A high polymer concentration and an increased ionic strength support ordered structures, while elevated temperatures favor disorder structures ; therefore, xanthan gum is a thermally responsive biopolymer . At low temperatures, the native state of xanthan gum shows an ordered and rigid conformation as a single helical or a double-strand helix stabilized by inter- and intramolecular hydrogen bonds. The ordered conformation of the xanthan molecule is semi-flexible with a hydrodynamic length ranging from 600 to 2000 nm and a hydrodynamic diameter of 2 nm . At elevated temperatures (≥60°C) [12, 16, 24] and low ionic strength, the native state, which displays an order state, transitions to a more flexible disordered-denatured state . Optical rotation measurements have demonstrated that xanthan gum dissolved in distilled water at 25°C displayed the nonordered conformation . However, a decrease in temperature (<40°C) [16, 24, 28] and the simultaneous increase in the ionic strength cause conformation reversal to a reordered-renatured state [11, 12, 13, 14, 15, 16, 17, 18, 19, 21, 22, 23, 27, 29, 30]. In saline solutions, monovalent or divalent cations (e.g., Na+ and Ca2+) condense on the ionized carboxyl moieties on the xanthan trisaccharide side chains, reducing repulsive forces between polymer chains. The side chains collapse down to the backbone causing conformation transition to a rigid rod-like shape of reduced hydrodynamic size stabilized by hydrogen bonding . This conformation increases the intra- and intermolecular attraction and the xanthan chains tend to adopt a more rigid ordered conformation [13, 14]. The stability of xanthan gum is attributed to its ordered conformation which is stabilized by salts. Thus, the optimum functionality of xanthan gum requires the addition of salt .
Xanthan gum is prone to self-association at low concentrations and has been used as a building block to generate self-assembled structures [24, 25]. The onset of macromolecular self-organization has been reported at concentrations ≥0.1 wt% . Parallel packing or side-by-side associations stabilized by hydrogen bonds facilitate the formation of three-dimensional networks [8, 19, 26]. Previous research has also demonstrated the self-organization of xanthan gum through polyelectrolyte complexation with other polysaccharides, such as chitosan-xanthan, β-lactoglobulin-xanthan, α-galactosidase-modified guar gum-xanthan, and sodium caseinate-xanthan, among many others [8, 26, 31]. Another example of self-aggregation through hydrophobic interactions is the intermolecular binding of xanthan gum-carob gum. These self-organizations take place in both the ordered and disordered conformations of the xanthan macromolecule depending on the ionic strength [8, 20, 32, 33].
Advantages of xanthan gum include non-toxicity, high water solubility, salinity tolerance, stability over a broad range of pH values, thermal stability against hydrolysis provided by its ordered conformation, high shear stability, high viscosities but a significant shear-thinning behavior on shearing at a low concentration, slight variations in viscosity with changes in temperature, availability, the ease of processing, and low manufacturing costs [11, 17, 18, 22, 26, 34, 35]. The main downside of xanthan gum is high sensitivity to microbial attack. Salt-tolerant aerobic and anaerobic microorganisms can degrade the xanthan gum chains leading to loss in solution viscosity. In practical applications, biocides are added to the xanthan gum solution to suppress the growth of degrading microorganisms [11, 17, 36].
Partially hydrolyzed polyacrylamides, HPAMs (Figure 1(b)), with degree of hydrolysis ranging from 25 to 35%, are the most used polymers for enhanced oil recovery (EOR) [35, 37]. HPAM is highly sensitive to mono- and divalent cation environments because of the shielding effect of the negative charges on the polymer backbone. Thus, the static repulsion between the HPAM lateral groups fades and the polymer structure collapses, which drastically reduces the viscosity of the polymer solution . Divalent cations (e.g., Ca2+) can also induce the self-aggregation of HPAM through polyion-cation complexation and depending on the concentration of Ca2+ inter- and intrachain complexation takes place . The molecular conformation and viscosity of HPAM solutions are also affected by the degree of hydrolysis, pH, temperature, molecular weight, pressure, and solvent quality [35, 36]. HPAM is susceptible to mechanical degradation under high shear due to chain scission reducing the polymer chain size and molecular weight, which in turns reduces the viscosity of the polymer solution. Advantages of HPAM are low manufacturing costs and resistance to bacterial attack .
Hydrophobically modified polyacrylamides (HMPAMs) are water-soluble polymers containing both hydrophobic groups (e.g., methyl or ethyl acrylates, alkyl vinyl ethers, styrene comonomers, or alkyl acrylamides) and weakly charged pendant groups (e.g., carboxylic acid pendant groups) directly attached to the polymer backbone (Figure 1(c)). The hydrophobic groups can be distributed in a block-like fashion, randomly, or discretely distributed along the backbone. In aqueous solutions, these hydrophobic groups aggregate through intra- and intermolecular associations that increase the hydrodynamic volume of the polymer, which increases the viscosity of the polymer solution [36, 38]. The alkyl chain length and charge density determine the hydrophobicity of these polymers . The presence of counter-ions in the aqueous media reduces the repulsion between charged groups within the polymer chain, which favors inter- and intrachain hydrophobic interactions [39, 40]. Benefits of HMPAM include salt tolerance and the enhancement in solution viscosity in the presence of low-molecular-weight electrolytes because of the shielding of intramolecular Coulombic attractions rather than the intermolecular hydrophobic interactions . The inter- and intramolecular hydrophobic interactions are dynamic and reversible. Therefore, under high shear rate, these associations are interrupted and the viscosity of the solution decreases, but as soon as the high mechanical shear is removed, the hydrophobic groups re-associate and the viscosity of the solution returns to its original value .
The goal of this exploratory research was to formulate a supramolecular polymer network with enhanced properties (i.e., viscoelasticity, mechanical stability, salt tolerance, and thermal stability), taking advantage of the synergistic combination of the beneficial properties of the individual polymers in the blend. The formation and characterization of the supramolecular polymer network was demonstrated through frequency (time) and temperature-dependent oscillatory rheology [4, 5]; the use of other analytical techniques for structural characterization of the supramolecular system is beyond the scope of this work.
In this chapter, the formulation and characterization of the supramolecular self-assembled polymer network (SAP) is first described, and then the effect of ionic strength on the viscoelastic behavior of the SAP is discussed. The next section describes the structural strength of the SAP through dynamic mechanical analysis (DMA), followed by the evaluation of the SAP thermal stability by dynamic mechanical thermo-analysis (DMTA). In the following section, the long-term thermal stability of the SAP prepared in brines having different ionic strengths is discussed. Finally, the performance of the SAP in displacing heavy oil employing conventional sad-pack displacement tests at simulated oil reservoir conditions is presented.
2. Formulation of the self-assembled polymer network (SAP)
Several types of polymers commercially available were evaluated for the formulation of the SAP network with enhanced viscoelastic flow behavior. Xanthan gum (B), commercial food grade (Groupe Maison Cannelle Inc. (Richmond, QC, Canada)), a partly hydrolyzed polyacrylamide, HPAM, with a degree of hydrolysis ranging from 5 to 10 mol% and a molecular weight of approximately 5 × 106 daltons  (GelTech, Midland, TX, USA), and AP of low anionicity, low-molecular weight (8–12 million Dalton), and a high hydrophobic content [42, 43, 44] (SNF Floerger, Riceboro, GA, USA). Baseline polymers and polymer blends were initially prepared in brine solution of 2.1 wt% concentration (see Table 1). Polymer solutions were mixed using a magnetic stirrer under strong mixing conditions to prevent the formation of lumps (e.g., fish eyes) at room temperature. The viscoelastic behavior, DMA, and DTMA of the baseline polymers and SAP were characterized through oscillatory rheology at 25°C using a Bohlin Geminin HR Nano Rheometer manufactured by Malvern (Worcestershire, UK) equipped with a parallel-plate measuring geometry (gap: 1000 μm) and a solvent trap to prevent drying effects during measurements. The amplitude sweep was performed in the strain range from 1 to 1000% at a fixed frequency of 1 rad/s, while the frequency sweep was run from 0.01 to 100 rad/s at fixed strain within the linear viscoelastic (LVE) range as determined from the preceding amplitude sweep.
|Brine compositions (wt%)|
Figure 2 displays the frequency sweeps as the curve functions of the loss factor (tan
The frequency sweeps (Figure 2) demonstrate that all polymers follow the characteristic shear-thinning flow behavior of polymers, thus viscosity decreases with increasing shear rate. At the same salinity (2.1 wt% brine), temperature, and angular frequency range, polymer B at 0.2 wt% solution concentration shows a significantly higher viscoelasticity than the HPAM at 0.2 wt% solution and the AP at 0.1 wt% solution. The behavior of polymer B (i.e., xanthan gum) results from its molecular-ordered aggregation behavior in saline solutions.
Regarding the loss factor (tan
The polymer blends (PBs) and respective concentrations evaluated were as follows:
All polymer blend solutions were homogeneous as such phase separation was not observed. The dynamic rheological properties of PB #1, #2, and #4 (Figure 3) suggest polymer interactions with an enhanced viscoelasticity relative to the baseline polymers, except for PB # 3 (
Polymer blend # 4 -
Supramolecular systems can be formed via electrostatic interactions due to the high solubility of charged groups in water. Previous research has demonstrated that xanthan gum and HPAM form physical networks through ionic cross-linking using divalent cations (e.g., Ca2+) [2, 26]. More examples of network systems built up through electrostatic interactions are reported in Ref. . Specifically, Ca2+ is an efficient binder for carboxylic acids that induce aggregation in aqueous polymer solutions through the formation of polyion/cation complexes. In these systems, “the focal point is the carboxylate moiety [that is an] excellent ligand” .
In this work, the anionic polymers were mixed in brine containing 3300 ppm of CaCl2 (see Table 1, brine 2.1 wt%). In this system, self-assembling is dominated by rapid cooperative electrostatic interactions in which the divalent cations, Ca2+, bridge the negative charges (i.e., carboxylic groups) in the polymer macromolecules causing complexation of a mixture of anionic polymers. In this case, the divalent cations act as the physical crosslink among the anionic polymer chains [6, 8]. The interpolymer associations driven by electrostatic interactions decrease the intra- and interpolymer electrostatic repulsion promoting the intra- and intermolecular hydrophobic interactions (i.e., van der Waals interactions) among the hydrophobic segments of the macromolecules forming a stronger network structure . Therefore, the screening of the charged groups by divalent cations reduces the steric hindrance among polymer chains and aids the interpolymer association via hydrogen bonding and hydrophobic interactions . Hydrogen bonding among side chains (e.g., carboxylic acids and amide groups) of polymers B, HPAM, and AP takes place, as previously demonstrated between HPAM and xanthan gum side groups [35, 51]. In solution, supramolecular networks are commonly controlled by strong intra- and intermolecular hydrogen bonds. “The double hydrogen bonding of two or more amides can work in a cooperative manner to drive the formation of many ordered supramolecular architectures” .
Figure 4 displays the frequency sweep rheometry data that shows the effect of varying the concentration of polymer B in PB # 1 and # 4 from 0.1 to 0.3 wt%, while maintaining the concentrations of HPAM and AP fixed at 0.2 and 0.1 wt%, respectively.
Increasing the concentration of polymer B significantly increases the elasticity and viscosity of both blends. However, the largest gain in viscoelasticity is shown by PB # 4. The rheological data suggest that increasing the concentration of polymer B encourages more intra- and interpolymer chain associations through cation bridging, hydrophobic interactions, and hydrogen bonding, which enhances the structural strength and viscosity of the SAP without compromising its solubility in brine solution . Furthermore, PB # 4 exhibits the lowest crossover point (
On the basis of the results obtained from oscillatory rheology in this exploratory research, a hypothetical structure of the optimum supramolecular polymer network is proposed in Figure 5, which shows the plausible reversible interactions taking place during self-aggregation of the SAP network.
Forthcoming research will characterize the structure of the optimum SAP system in depth, employing several analytical techniques (i.e., 1H Nuclear Magnetic Resonance (1H-NMR), Scanning Electron Microscopy (SEM), Fourier Transform Infrared Spectrometry (FTIR), and Size Exclusion Chromatography, among others) to test the proposed hypothetical SAP structure shown in Figure 5. In the succeeding section, a qualitative characterization of the polymers and SAP morphologies was conducted through optical microscopy. However, a more comprehensive characterization of these systems is required. This information will be provided in the upcoming work, which is beyond the scope of this chapter.
The morphology of the baseline polymers samples and the optimum SAP was observed using a polarized light optical microscope (Olympus model GX41), equipped with an M Plan N 10×/0.25 ∞/-FN22n objective (Olympus), digital camera, and image analysis software (Lumenera model Infinity 2-2C). Figure 6(a) and (b) display the micrographs of the baseline polymers and SAP dissolved in distilled water and in brine (8.4 wt%), respectively. In these micrographs, Figures 1–4 correspond to polymers AP, B, HPAM, and SAP respectively.
In the photomicrographs presented in Figure 6(a) is possible to qualitatively observe the morphology of the different polymer systems despite light interference . The micrograph of the AP polymer in distilled water (Figure 6(a1)) reveals well-separated ramifications of aggregated macromolecules or clusters as previously reported for hydrophobically modified polyacrylamides [6, 40], while polymer B (Figure 6(a2)), HPAM (Figure 6(a3)), and the SAP (Figure 6(a4)) display extended macromolecular configurations. The polymer blend in Figure 6(a4) exhibits a more dense, well-aligned, and extended configuration of polymer structures. This macromolecular configuration results from the reciprocal charge repulsion among the anionic polymers stretching out the chains, which occupy a larger hydrodynamic volume because, minimum interchain interactions take place in distilled water [13, 26].
Figure 6(b1)–(b4) demonstrate that in brine solution, the screening of the negative charges in the polymer chains causes the increase of intra- and interchain interactions among the anionic polymers. For instance, dense intra- and interchain hydrophobic interactions are visible for the associating polymer, AP, in Figure 6(b1), in the form of a dense network that was not observed in distilled water (Figure 6(a1)). Micrographs in Figure 6(b2) and (b3) display branch-like fractal structures for polymer B and HPAM, which agree with previous research . The screening of the negative charges in the polymer side chains causes the coiling/folding of the polymer chains that decreases the hydrodynamic volume of the macromolecules and the viscosity of the polymer solutions [13, 26]. By contrast, Figure 6(b4) exposes a network of fully entangled macromolecules. This high-density thread-like net reveals a homogeneous web of intra- and interchain interactions among the anionic polymers.
3. Effect of ionic strength on the viscoelasticity of the SAP system
Three brine concentrations 2.1, 4.2, and 8.4 wt% (see Table 1) were employed to establish the effect of ionic strength on the viscoelasticity of the SAP system. Figure 7 presents the frequency sweep of the SAP and baseline solutions in different brine concentrations in terms of the curve functions of tan
Figure 7 demonstrates the significant effect of ionic strength on the SAP system. At the highest ionic strength (i.e., brine 8.4 wt%), the SAP system displays the highest elasticity and viscosity. The curves in Figure 7 show
These rheological data indicate that the higher the ionic strength the higher the suppression of the electrostatic repulsion among polymer chains through cation bridging (i.e., Ca2+), which results in more and stronger intra- and specially interpolymer complexations and associations that reinforce the polymer network and enhances the viscosity of the solution . Previous research has also demonstrated that the addition of inorganic salts to interpolymer mixtures (e.g., anionic and nonionic polymers) in aqueous solutions deteriorates the thermodynamic quality of the solvent (e.g., water) with respect to the polymers, which promotes the strengthening of the interchain complexation through hydrophobic interactions and hydrogen bonding .
The main difference between the SAP system and the baseline shown in Figure 7 is that the SAP system contains 0.1 wt% of AP polymer (i.e., hydrophobically modified polymer); therefore, the addition of inorganic salts shelters the charged groups in the associating polymer side chains and uncovers the hydrophobic moieties, making these associating groups more accessible for intra- and interpolymer hydrophobic interactions [31, 36]. These observations agree with previous work .
These experimental findings indicate that the viscoelastic functionality of the SAP formulation is improved as the ionic strength in the aqueous solution increases. This performance makes the SAP system suitable for EOR applications involving brines containing high salinity and hardness concentrations.
4. Dynamic mechanical analysis (DMA)
The structural strength of a material is usually determined through the reestablishment of the storage modulus,
Figure 8 displays the curves of
Figure 8 shows that at low salinity (i.e., brine 2.1 wt%), the baseline displays a complete structural regeneration (i.e., thixotropic behavior), while the SAP system exhibits a 5% increase in the structural strength relative to the reference value of
At high brine concentration (i.e., 8.4 wt%), the baseline does not show complete structural regeneration (Figure 8). The
These results verify the reversibility of the interpolymer interactions of the SAP system involving the instant recovery of the noncovalent associations following shear thinning . This demonstrates the self-healing advantage of supramolecular polymer networks due to the reversibility of the physical associations and high-chain mobility in water [3, 6, 58].
5. Dynamic mechanical thermo-analysis (DMTA)
Dynamic mechanical thermo-analysis was conducted by performing upwards temperature ramps from 282.5 (9°C) to 353.5 K (80°C) at a linear heating rate of 9 K/min and downwards temperature ramps from 353.5 (80°C) to 282.5 K (9°C) at a linear cooling rate of 7 K/min at a constant frequency (1 Hz) and % strain (20%) within the LVE range. Figure 9 displays the oscillatory upward and downward temperature sweeps showing the
The upward heating curves (Figure 9) show that for both systems (i.e., baseline and SAP network), the
Figure 10 shows that the baseline system reaches the gel transition temperature (
The SAP system displays a different behavior as shown in Figure 10. In both brine salinities (2.1 and 8.4 wt%), the heating curves do not reach the gel transition temperatures. At low salinity, the cooling curve just reaches the crossover point (G’ = G” and tan
6. Extended thermal stability
The extended thermal stability evaluation was performed at 90°C for a period of 8 weeks. Figure 11 displays the
The thermal deterioration of the viscoelasticity of both systems as a function of time could be attributed in part to the autohydrolysis of the amide moieties (i.e., acrylamide groups) and hydrophobic functional groups forming additional acrylate moieties at elevated temperatures (i.e., >85°C). These acrylate structures rapidly associate with divalent cations (i.e., Ca2+) causing the precipitation of polymer from the bulk of the solution, which becomes turbid. More detailed information on autohydrolysis of polymers at elevated temperature and ionic strength is provided elsewhere [43, 59]. Thermal degradation of the polymer samples can also be attributed to the induced breaking of the acrylic backbone trigger via free-radical reactions, which reduces the molecular weight of the polymer chains .
Although this extended thermal stability evaluation demonstrates the significant effect of temperature and time on the viscoelastic
7. Heavy oil recovery
The performance of the baseline and the SAP system as mobility control agents in displacing and mobilizing heavy oil was carried out through conventional sand-pack displacement tests. The heavy oil that was provided by Husky Energy Inc. (Calgary, AB, Canada) had an initial viscosity of 68,728 cP at 25°C that was adjusted to 3000 cP at 25°C by dilution with natural condensate (density: 0.9 g/ml) provided by Corridor Resources Inc. (McCully field, Sussex, NB, Canada). A Temco DCHH-series core holder (Temco Inc., Tulsa, OK, USA) was employed to perform the displacement tests. The core holder’s rubber sleeve was packed with sand (QUIKRETE® Premium Play Sand®, No. 1113, 100% quartz) of effective size: D10 = 180 μm and a uniformity coefficient: D60/D10 = 2.44 determined by sieve analysis (ASTM C136/C136M-14)  employing woven wire brass sieves (Endecotts Limited, London, UK). The packed sleeve was sealed using the floating distribution plug and inserted into the core holder body. An overburden pressure of 500 psi was applied by filling the annulus between the outer diameter of the sleeve and the inner diameter of the core holder body with distilled water. CFR-series transfer vessels (Temco Inc., Tulsa, OK, USA) were used to store heavy oil, brine, and polymer that were pumped to the sand pack by a Teledyne ISCO Syringe pump, model 100DX (Teledyne Isco Inc., Lincoln, NE, USA). Pressure gauges (Omega, Laval, QC, Canada) with an accuracy of 0.5% (FS) were installed in different sections of the sand-pack displacement setup (Figure 12).
Four displacement tests were carried out at 25°C. Two displacement tests evaluated the performance of the baseline system and the other two tests the performance of the SAP network. The unconsolidated porous media were characterized by determining the pore volume (PV), porosity (
|Flooding test #||Pore volume, PV (cm3)||Porosity, ||Permeability, |
|Baseline # 1||208||29||10,049|
|Baseline # 2||206||29||8667|
|SAP # 1||204||29||8109|
|SAP # 2||187||26||4700|
The fluid injection sequence was carried out in four steps as follows. The first step was the injection of heavy oil into the brine-saturated porous media until no more brine was produced from the sand pack that corresponded to approximately two pore volumes (2PV), followed by the second step of brine (8.4 wt%) injection to displace heavy oil (i.e., water flooding) until the production of oil stopped, which corresponded on average to the injection of 6 PVs of brine. The third step consisted of the injection of 1 PV of baseline and/or the SAP system as EOR mobility control agents to further displace and recover oil. The fourth and final step was the post-polymer brine (8.4 wt%) injection as a chaser to displace the baseline polymer and/or the SAP system through the sand pack. On average, 6PV of post-polymer brine was injected. The average injection flow rate was 0.76 ml/min that corresponds to a linear velocity of 0.77 ft./day. During each injection step, the volume of fluid injected, the volume of fluid produced, injection time, and pressures at the inlet, at the sand-pack pressure ports, and outlet of the sand-pack holder were recorded. Material balance of each injection step was carried out to determine the sand-pack fluid saturation and oil recovery. More details on the experimental procedure employed during these routine sand-pack displacement tests are provided in Ref. .
The performance of the baseline and the SAP network as mobility control agents in porous media was analyzed by plotting the effective viscosity or resistance factor (RF) [63, 64, 65, 66, 67, 68] of the polymer system during flow through porous media as a function of the volume of fluid injected expressed as a fraction of pore volume (PV), which was normalized for porosity and permeability to compare the displacement tests on the same reference. The capillary bundle parameter model was applied for data normalization [66, 69, 70, 71].
Polymer retention in porous media after the post-polymer brine injection was determined by the residual resistance factor, RRF [59, 62, 63, 64, 65, 67, 68, 70, 71, 72, 73, 74]. RF and RRF are significant parameters because they provide reliable information on the propagation and effectiveness of polymeric systems as mobility control agents through porous media. Figure 13 displays the average RF and RRF as a function of the volume of fluid injected normalized for porosity and permeability of the baseline and the SAP system sand-pack displacement tests.
The RF curves reveal that the SAP system offers a higher end value of effective viscosity, RF (61%), during flow in porous media relative to the baseline. The SAP RF curve also shows a tendency to level off as a function of the volume of fluid injected, which indicates an appropriate propagation of the SAP network through the unconsolidated porous media. Therefore, the SAP network displays a better performance as mobility control agent compared with the baseline system.
The RRF curves indicate a larger retention of the SAP system along the sand pack with an end RRF value that stabilizes at around 2.8, while the end RRF value induced by the baseline levels off at approximately 1.3. Therefore, the permeability of the unconsolidated sand packs was further reduced by the SAP system, which aids the displacement and mobilization of heavy oil by further reducing the relative permeability to water [70, 75].
Figure 14 shows cumulative oil recovery as the percentage of the original oil in place (OOIP) recovered, the ratio of the remaining oil saturation to the initial oil saturation (
Polymer-flooding and the post-polymer water-flooding steps rendered an overall percentage of cumulative oil recovery of 41% for the baseline system and 51% for the SAP network. Therefore, the SAP system rendered a 10% higher incremental oil recovery relative to the baseline. In field applications of polymer flooding, an incremental oil recovery of 5% is considered successful .
The superior performance of the SAP network in displacing heavy oil is attributed to an enhanced effective viscosity during flow in porous media, which generates a more stable displacement front that increases the volumetric sweep efficiency accelerating the production of oil. Besides, both systems—the baseline and the SAP network—show to be very efficient in controlling WOR during the polymer-flooding stage. However, as soon as the post-polymer water flooding is initiated, the water to oil ratio, WOR, increases very rapidly, due to the uncontrollable channeling of brine toward the production end caused by viscous fingering .
A stable supramolecular system was formulated based on the self-assembling of xanthan gum, HPAM, and HMPAM driven by electrostatic interactions through divalent cation (i.e., Ca2+) bridges, which reduce the steric hindrance among anionic polymer chains promoting strong and stable intra- and interpolymer associations via hydrophobic interactions and hydrogen bonding. The viscoelastic functionality of the SAP system is enhanced in high ionic strength aqueous solutions. This performance makes the SAP system suitable for EOR applications involving brines containing high salinity and hardness concentrations.
The SAP system shows a high structural strength, mechanical stability, and self-healing capabilities. The supramolecular polymer network exhibits instant recovery of the interpolymer noncovalent interactions and even the increase in structural strength following the lifting of high-shear conditions (i.e., severe shear thinning).
In the temperature range from 282.5 (9°C) to 353.5 K (80°C), the SAP network exhibits thermal stability. In this temperature range, the strong and stable intra- and interchain interactions maintain the integrity of the supramolecular polymer and its flow viscoelastic behavior. Likewise, the SAP system demonstrated an enhanced thermal stability after 8 weeks at 90°C in high-salinity brine (8.4 wt%) compared with the thermal performance of the baseline. This further confirms that the functionality of the SAP system is upgraded at higher ionic strengths due to the formation of stronger intra- and interpolymer associations.
The SAP system rendered a 10% higher incremental oil recovery relative to the baseline system. The superior performance of the SAP network in displacing heavy oil is attributed to better mobility control properties, to the generation of a stable displacement front, the efficient and rapid control of the WOR, and an improved volumetric sweep efficiency that accelerates the production of oil. Overall, the SAP system is a straightforward formulation that offers several advantages relevant to EOR such as enhanced viscoelastic flow behavior, increased functionality in high ionic strength environments, stability to mechanical shear, and an improved thermal stability.
The authors would like to extend their appreciation to Dr. Chutima Kongvarhodom, Department of Chemical Engineering, Faculty of Engineering, King Mongkut’s University of Technology Thonburi (KMUTT), Thoongkru, Bangkok, Thailand, for leading the academic exchange program between KMUTT and the University of New Brunswick (UNB). Likewise, the authors gratefully acknowledge GelTech, SNF Floerger, Husky Energy, and Corridor Resources Inc. for providing samples of polymers, heavy oil, and condensate. The authors would like to acknowledge financial support from the UNB through the Sabbatical Research Grant and the Canada Foundation for Innovation, CFI, research grant.